2650 A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655stants, low dielectric loss, nearly zero resonance frequency Table 1temperature coefﬁcient and low sintering temperature, will Relative densities of doped BZN samples sintered at different temperatures.enhance the application areas of these ceramics. Different meth- Relative density (%)ods can be used in order to enhance the properties of BZN 0.2 mol% 0.5 mol% 1.0 mol% 2.0 mol% 4.0 mol% Sinteringdielectric ceramics. Some of these methods are, employment of temperaturechemical methods, addition of low melting temperature-glassy In 91.86 97.59 97.99 99.67 99.79 1300 ◦ Cphases, and doping. Ce 97.85 95.25 96.71 96.95 92.84 1400 ◦ C In this paper, In, Ce and Bi doped Ba(Zn1/3 Nb2/3 )O3 (BZN) Bi 94.68 91.44 90.70 95.92 95.87 1250 ◦ Cceramics were prepared by conventional mixed oxide technique.The effect of each dopant on the sintering temperature and Theoretical density of undoped BZN ceramic is 6.516 g/cm3 .dielectric properties were investigated. In, Ce and Bi doped BZNceramics were characterized by XRD and SEM. where αε , temperature coefﬁcient of dielectric constant; εT2 , dielectric constant at 120 ◦ C; εT1 , dielectric constant at 20 ◦ C;2. Experimental details T2 = 120 ◦ C; T1 = 20 ◦ C. Powders of BaCO3 (Fluka; >98.5%), ZnO (Sigma–Aldrich; 3. Results and discussion99%) and Nb2 O5 (Alfa Aesar; 99.9%) were mixed in stoichio-metric proportion in ethanol medium in a plastic container for 3.1. Densities of doped BZN ceramics20 h. After drying the slurries at 100 ◦ C for 24 h, they were milledin an agate mortar and calcined at 1100 ◦ C for 4 h in a closed In doping into the BZN improved the sintering of BZN ceram-crucible. Oxides of dopant (In2 O3 , 99.9% Alfa Aesar; Bi2 O3 , ics. Densities of In-doped BZN samples sintered at 1300 ◦ C99.9%, Acros; CeO2 , 99.9%, Acros) additives were added in the for 4 h increased with In content in the range of 0.2–4.0 mol%molar ratios of 0.2%, 0.5%, 1.0%, 2.0%, 4.0% into the fabricated (Table 1). Although 0.2 mol% In doped BZN had a 92% ofBZN powders and the mixtures were ball milled again in ethanol relative density, 4.0 mol% of In doping resulted in ∼99% offor 20 h. The slurry was dried and milled in the agate mortar and relative density. Increasing sintering temperatures raised thepressed into pellets with 10 mm diameter and 1–2 mm thickness densities of In doped BZN samples even at low doping con-by a uniaxial press with 2 MPa pressure. The pellets were buried centrations. 0.2 mol% In-doped BZN had a relative density ofin the BZN powder and sintered at different temperatures in a 97% at sintering temperature of 1500 ◦ C. Dense Ce-doped BZNhigh temperature furnace for 4 h in a tightly closed alumina cru- ceramics were produced by 0.2 mol% of Ce doping at lowercible to minimise the loss of volatile species. High temperature temperatures like 1250 ◦ C. Nevertheless, as the Ce-doping con-furnace was heated to 1250–1500 ◦ C at of 250 ◦ C/h, and samples centration increased, the densities of Ce-doped BZN pelletswere cooled from sintering temperature to 900 ◦ C at 120 ◦ C/h decreased. Therefore, the density of Ce-doped BZN ceramicsand to room temperature at 250 ◦ C/h. with amount of dopants was evaluated at 1400 ◦ C. High relative Surfaces of the pellets were grinded to ensure proper density density of around 98% was obtained at 0.2 mol% Ce but themeasurements. Bulk densities of the samples were measured density decreased to 92% at 4 mol% of Ce. This could be due toby Archimedes method. The theoretical densities of the doped formation of secondary phases as inclusions in the microstruc-BZN samples were calculated using the respective lattice param- ture of BZN as supported by SEM. The density of Bi-doped BZNeters of each sample calculated by X-ray diffraction. The phases samples sintered at 1250 ◦ C for 4 h did not change consistentlywere characterized by X-ray diffractometry with Cu K␣ radia- with the amount of Bi. Although 94.5% of relative density wastion (λ = 1.5418 A) in the range 2θ: 20–70◦ . The fracture surfaces ˚ achieved at 0.2 mol% of Bi, the density decreased ∼4% at 0.5of the specimens were examined in the SEM at 20 kV after coat- and 1 mol% and again increased to 95.9% at 2.0 and 4.0 mol%ing with Au/Pd alloy by sputter coater. Chemical analysis was of doping. The sharp decrease in density at 0.5 mol% dopingconducted by means of dispersive spectrometry (EDS) in the could be due to formation of secondary phases as suggested bySEM. XRD. Although XRD of 1.0 mol% Bi-doped BZN did not give Pellets with a relative density over 97% have been used for any secondary phases, the density decrease at 1.0 mol% could bedielectric measurements. The circular faces of the dense and possibly due to secondary phases which could not be detected bysingle phase pellets were painted with silver paste using vacuum XRD due to its high detection limit. Around 96% of relative den-coating system, then copper leads were attached on the surfaces sity was obtained in samples doped with 2.0 and 4.0 mol% Bi.using silver and disks were dried in an air oven. These disks Higher sintering temperatures above 1250 ◦ C to obtain higherwere used for dielectric measurements. The dielectric constant densities led to melting of samples.and dielectric loss were measured using LCR meter in the lowfrequency range from 1 kHz to 2 MHz between 20 and 200 ◦ C. 3.2. XRDThe temperature coefﬁcient of dielectric constant was calculatedby the following formula: XRD of In-doped BZN ceramics showed single phase per- ovskite structure for all In doping contents ranging between 0.2 εT2 − εT1 and 4.0 mol% at sintering temperature of 1300 ◦ C. No additionalαε = εT1 (T2 − T1 ) peaks on the XRD pattern were observed after doping indicating
A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655 2651the absence of secondary phases (Fig. 1). Ce-doped BZN ceram-ics sintered at 1400 ◦ C for 4 h also produced single phase BZNand no secondary phases were detected. In order to investigatethe effect of sintering temperature on the phase development,0.5 mol% Ce doped BZN was sintered between 1150 ◦ C and1450 ◦ C for 4 h (Fig. 2). At 1150 ◦ C, there were secondary phasesin addition to BZN and their amounts decreased with sinteringtemperature ﬁnally giving single phase at 1300 ◦ C. Sinteringat higher temperatures above 1400 ◦ C gave no dissociation ofBZN or any other secondary phases. These results indicatedthat BZN formation depends strongly on temperature and hightemperatures were required to obtain single phase BZN. XRD ofBi-doped BZN samples sintered at 1250 ◦ C showed single phase Fig. 3. XRD patterns of 0.2, 0.5, 2.0 and 4.0 mol% Bi-doped BZN ceramicsperovskite structure for all doping contents except for 0.5 mol% sintered at 1250 ◦ C for 4 h (p = BZN phase).doping (Fig. 3). Since XRD of 0.5 mol% Bi doped BZN sinteredat 1250 ◦ C gave secondary phases, it was sintered at various tem-peratures for 4 h to obtain single phase at higher temperatures.Although at 1200 ◦ C there were high amounts of unidentiﬁedsecond phases, they disappeared completely at 1300 ◦ C givingsingle phase (Fig. 4). This revealed that sintering temperatureof 1250 ◦ C was not enough for the formation of single phaseBZN when Bi doping amount was 0.5 mol%. However, it wasnot understood that same kind of behaviour was not observed Fig. 4. XRD patterns of 0.5 mol% Bi doped BZN ceramics sintered at various temperatures for 4 h (p = BZN phase, * = unidentiﬁed phase). for the other doping contents which gave single phase at 1250 ◦ C. 3.3. Lattice parametersFig. 1. XRD patterns of 0.2, 0.5, 1.0, 2.0 and 4.0 mol% In-doped BZN ceramicssintered at 1300 ◦ C for 4 h (p = BZN phase). Avarage lattice parameters of doped BZN samples are given in Table 2. In and Ce dopings generally increased the lattice parameter of BZN. The increase in lattice parameter was due to the greater ionic radius of In3+ and Ce4+ than that of Zn2+ (Table 3). It was thought that In and Ce dopants replaced the Zn cation in the BZN structure and formed substutional solid solution and therefore they resulted in an increase in the lat- tice parameter. On the other hand, Bi doping did not cause a Table 2 Lattice parameters of doped BZN samples. Lattice parameter (Å) 0.2 mol% 0.5 mol% 1.0 mol% 2.0 mol% 4.0 mol% Sintering temperature In 4.0941 4.0962 4.1008 4.1155 4.1202 1300 ◦ C Ce 4.1369 4.1379 4.1434 4.1437 4.1543 1400 ◦ C Bi 4.0913 4.0893 4.0862 4.0922 4.0935 1250 ◦ CFig. 2. XRD patterns of 0.5 mol% Ce-doped BZN ceramics sintered at varioustemperatures for 4 h (p = BZN phase; * = unidentiﬁed phase). ˚ Lattice parameter of undoped BZN ceramic is 4.09408 A.
2652 A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655Table 3 3.4. SEMIonic radii values of dopants and Ba, Zn, Nb cations depending on coordinationnumbers. SEM of 0.5 and 4.0 mol% Bi doped BZN ceramic showedElement Coordination number Ionic radius (Å) only single phase BZN (Fig. 5). No secondary phase wasBa 8 1.42 detected, as observed by XRD. It can be seen from the ﬁgures 12 1.61 that as the Bi doping content increased the perovskite grain sizeZn 6 0.74 signiﬁcantly increased which could be due to formation of liquid 8 0.90 phases at high Bi content. EDS analyses taken from grains indi-Nb 6 0.64 cated identical composition with theoretical BZN compositionIn 6 0.81 (Fig. 5c). Although XRD results showed that even 4.0 mol% of CeO2Ce 6 0.87 8 0.97 dissolved within BZN, SEM investigation indicated some sec- ondary phases even at 0.2 mol% Ce doping (Fig. 6). Some needleBi 6 1.03 8 1.17 like grains which were identiﬁed as barium oxide phase by EDS were observed in the microstructure of 0.2 mol% doped BZN (Fig. 6c). When Ce amount increased to 4.0 mol%, bar-consistent increase or decrease with doping content possibly ium oxide phase disappeared in the microstructure but a Ce-richdue to the formation of second phases as detected by XRD in phase occurred (Fig. 7). Ce-rich phase generally occurred as0.5 mol% Bi doped BZN sintered at 1250 ◦ C or due to the evapo- small inclusion particles either at grain boundaries or withinration of bismuth oxide and/or zinc oxide4,9–11 which may cause the grains. Comparing the microstructure of 0.2 and 4.0 mol%nonstoichiometric phases. Slight weight losses were observed Ce doped BZN ceramics, it is obvious that perovskite grains inin ceramics after sintering which indicates evaporation from the later case were much bigger. A small amount (0.2 mol%) ofmaterial. Ce doping signiﬁcantly reduced the grain size but a consider-Fig. 5. SEM micrographs and EDS analysis of Bi-doped BZN ceramics sintered at 1250 ◦ C for 4 h. (a) SEM micrograph of 0.5 mol% Bi2 O3 , (b) SEM micrographof 4.0 mol% Bi2 O3 and (c) EDS analysis from perovskite grains.
A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655 2653Fig. 6. SEM micrographs and EDS analysis of 0.2 mol% Ce-doped BZN ceramic sintered at 1400 ◦ C for 4 h. (a) SEI at 10,000×, (b) SEI at 5000×, (c) EDS analysisfrom barium oxide phase (point 1) and (d) EDS analysis from perovskite grains (point 2).able grain growth was observed at higher Ce-doping (4.0 mol%), 3.5. Dielectric measurementsprobably due to a liquid phase occurring during sintering at highCe content and/or due to the large distortion of the surrounding Compared with undoped BZN ceramic, In and Ce dopingslattice that facilitates defect migration.12,13 into the BZN generally increased the dielectric constant of BZNFig. 7. SEM micrograph and EDS analysis of 4.0 mol% Ce-doped BZN ceramic sintered at 1400 ◦ C for 4 h. (a) SEI at 5000× and (b) EDS analysis from Ce-richphase (point 1).
2654 A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655Fig. 8. Variation of dielectric constant (DC) and temperature coefﬁcient of dielectric constant (TC) of (a) In doped, (b) Ce doped and (c) Bi doped BZN as a functionof dopant content at 25 ◦ C, at 1 MHz.(Fig. 8). While Ce doping increased the dielectric constant from observed by SEM (Figs. 6 and 7). Bi doping into the BZN also41 to over 66, Ce doping increased it from 41 to around 60. caused a general increase in dielectric constant (from 41 to 63)The increase in dielectric constant could be due to higher polar- which could be due to higher densities of BZN at higher Bi dop-izability of In and Ce than that of Zn (Zn: 7.1 × 10−24 cm3 ; ings. Temperature coefﬁcient of dielectric constant increasedIn: 10.2 × 10−24 cm3 ; Ce: 26.6 × 10−24 cm3 ).14 Temperature to around 151 ppm/◦ C at 0.5 mol% Bi and then decreased withcoefﬁcient of dielectric constant decreased with increasing In Bi doping reaching to a value of −81 ppm/◦ C at 4.0 mol% Bi.doping until 1.0 mol% In giving temperature coefﬁcient of Although XRD and SEM of Bi doped BZN indicated only sin-−469 ppm/◦ C but then it increased to around −54 ppm/◦ C above gle phase, the decrease in temperature coefﬁcient could be due1.0 mol% doping (Fig. 8). The sharp decrease in temperature to secondary phases which could occur at grain boundaries orcoefﬁcient at 1.0 mol% In could be due to formation of remnant grain junctions in low amounts that cannot be detected by SEM.impurity phases which could not be detected in SEM. Ce doping The change in dielectric constant and dielectric loss of In,into the BZN structure decreased the temperature coefﬁcient of Ce and Bi doped BZN ceramics were investigated as a func-dielectric constant giving a minimum value of −91 ppm/◦ C at tion of frequency and temperature. Doped ceramic had identical2.0 mol% Ce (Fig. 8). The decrease in temperature coefﬁcient behaviours. Fig. 9 shows the change of dielectric properties ofcould be due to increase in the amount of secondary phases as 2.0 mol% Ce doped BZN with frequency and temperature. It Fig. 9. Change of dielectric properties of 2.0 mol% Ce doped BZN with frequency and temperature (a) dielectric constant and (b) dielectric loss.
A. Mergen, E. Korkmaz / Journal of the European Ceramic Society 31 (2011) 2649–2655 2655was observed that the dielectric constant did not change consid- under the Project grant number 107M372 and Marmara Uni-erably with increasing frequency and temperature, as it varied versity Scientiﬁc Research Committee for ﬁnancial support ofjust between 59.9 and 60.2. Temperature had a more pronounced this investigation (FEN-E-040310-0040).effect than frequency. The dielectric loss slightly decreasedwith increasing frequency probably due to increase in leakage Referencescurrent.15,16 Although dielectric loss of Ce-doped BZN was notdependent on temperature between 20 and 100 ◦ C at all fre- 1. Sebastian MT. Dielectric materials for wireless communication. 1st ed.quencies, it was signiﬁcantly changed with temperature above Oxford: Elsevier; 2008.100 ◦ C at low frequencies (below 100 kHz). Dielectric losses of 2. Endo K, Fujimoto K, Murakawa K. Dielectric properties of ceramics in Ba(Co1/3 Nb2/3 )O3 –Ba(Zn1/3 Nb2/3 )O3 solid solution. J Am Ceram Socdoped BZN ceramics were generally below 0.015 and it gen- 1987;70:C215–8.erally raised with temperature possibly due to increase in the 3. Matsumoto K, Tamura H, Wakino K. Ba(Mg Ta)O3 –BaSnO3 high-Qnumber of charge carriers.17 dielectric resonator. Jpn J Appl Phys 1991;30:2347–9. 4. Desu SB, O’Bryan HM. Microwave loss quality of Ba(Zn1/3 Ta2/3 )O34. Conclusion ceramics. J Am Ceram Soc 1985;68:546–51. 5. Onoda M, Kuwata J, Kaneta K, Toyama K, Nomura S. Ba(Zn1/3 Nb2/3 )O3 –Sr(Zn1/3 Nb2/3 )O3 solid solution ceramics with In the current study, BZN ceramics doped with In, Ce and temperature stable, high dielectric constant and low microwave loss. JpnBi with the molar ratios of between 0.2 and 4.0 mol% were pro- J Appl Phys 1982;21:1707–10.duced by mixed oxide technique. XRD examinations of doped 6. Ioachim A, Toacsan M, Banciu MG, Nedelcu L, Stoicaa G. ZST type mate-ceramics indicated that In and Ce doped ceramics sintered at rial for dielectric resonators and substrates for hybrid integrated circuits. J1300 and 1400 ◦ C, respectively, gave single phase. But, Bi doped Optoelectron Adv Mater 2003;5:1395–8. 7. Varma MR, Sebastian MT. Effect of dopants on microwave dielectric prop-BZN sintered at 1250 ◦ C gave secondary phases at 0.5 mol% Bi, erties of Ba(Zn1/3 Nb2/3 )O3 ceramics. J Eur Ceram Soc 2007;27:2827–although single phase BZN was obtained at the other doping 33.contents. Sintering temperature had a substantial effect on the 8. Moulson AJ, Herbert JM. Electroceramics-materials-properties-BZN single phase formation. While the densities of In doped applications. 2nd ed. England: John Wiley and Sons; 2003. 9. Kawashima S, Nishida M, Ueda I, Ouchi H. Ba(Zn1/3 Ta2/3 )O3 ceram-BZN ceramics increased with In doping, increase in Ce doping ics with low dielectric loss at microwave frequencies. J Am Ceram Socled to a decrease in density of BZN due to formation of secondary 1983;66:421–3.phases. SEM investigation revealed that increase in Bi and Ce 10. Moussa SM, Ibberson RM, Bieringer M, Fitch AN, Rosseinsky MR. In situdoping contents increased the BZN grain size probably due to measurement of cation order and domain growth in an electroceramic.formation of a liquid phase. Although SEM of Bi doped BZN Chem Mater 2003;15:2527–33.revealed only single phase, Ce doping resulted in formation of 11. Mergen A, Lee WE. Fabrication and crystal chemistry of Bi3/2 ZnSb3/2 O7 pyrochlore. J Eur Ceram Soc 1996;16:1041–50.BaO second phase at low Ce doping and Ce-rich phase at high Ce 12. Chen PL, Chen IW. Grain growth in CeO2 : dopant effects, defect mecha-doping. In, Ce and Bi dopings generally increased the dielectric nism, and solute drag. J Am Ceram Soc 1996;79:1793–800.constant possibly due to the greater polarizabilities of the dopant 13. Zhang T, Hing P, Huang H, Kilner J. Densiﬁcation, microstructure andcations than the host cations. For all dopings, it was observed grain growth in the CeO2 –Fe2 O3 system (0 ≤ Fe/Ce ≤ 20%). J Eur Ceramthat dielectric constant did not change signiﬁcantly with increas- Soc 2001;21:2221–8. 14. Shannon RD. Revised effective ionic radii and systematic studies ofing frequency but temperature had a more pronounced negative interatomic distances in halides and chalcogenides. Acta Crystallogreffect on dielectric constant which decreased with temperature 1974;A32:751–67.increase. The dielectric loss of doped BZN ceramics generally 15. Wang H, Peng Z, Du H, Yao T. Mn4+ & W6+ substitution ondecreased at high frequencies. Bi2 O3 –ZnO–Nb2 O5 -based low ﬁring ceramics. Ceram Int 2004;30:1219– 23. 16. Lines ME, Glass AM. Principle and applications of ferroelectric materials.Acknowledgements Oxford: Clarendon Press; 1977. 17. Nobre MAL, Lanfredi S. Dielectric properties of Bi3 Zn2 Sb3 O14 ceramics We would like to give our great thanks to The Scientiﬁc at high temperature. Mater Lett 2001;47:362–6.and Technological Research Council of Turkey (TUBITAK)